Reduced Chemical Warfare Agent Sorption in Polyurethane-Painted Surfaces via Plasma-Enhanced Chemical Vapor Deposition of Perﬂuoroalkanes Wesley O. Gordon,*,†,‡ Gregory W. Peterson,†,‡ and Erin M. Durke§,† ‡
U.S. Army Edgewood Chemical Biological Center, 5183 Blackhawk Road, Aberdeen Proving Ground, Maryland 21010, United States § Excet, Inc., 8001 Braddock Road, Suite 303, Springﬁeld, Virginia 22151, United States S Supporting Information *
ABSTRACT: Perﬂuoralkalation via plasma chemical vapor deposition has been used to improve hydrophobicity of surfaces. We have investigated this technique to improve the resistance of commercial polyurethane coatings to chemicals, such as chemical warfare agents. The reported results indicate the surface treatment minimizes the spread of agent droplets and the sorption of agent into the coating. The improvement in resistance is likely due to reduction of the coating’s surface free energy via ﬂuorine incorporation, but may also have contributing eﬀects from surface morphology changes. The data indicates that plasma-based surface modiﬁcations may have utility in improving chemical resistance of commercial coatings.
KEYWORDS: chemical warfare agent resistance, plasma treatment, paint, polyurethane
enclosed by organic material. Post treatment, the pigments and ﬁllers are more exposed, likely due to etching away of the organic component of the paint. This likely increases the roughness of the surface of the paint on the submicrometer scale, which may decrease wetting properties of the surface with respect to water and other chemicals. In addition to SEM images, the treated and untreated panels were analyzed by confocal optical proﬁlometry to determine if there was any observable macroscopic (0.05−1 mm) scale changes in the paint morphology and roughness. No clear diﬀerences were observed (Figure S2 in the Supporting Information). X-ray photoelectron spectroscopy (XPS) was also performed on untreated and treated paint panels. The results in Table 1 and Figure S8 in the Supporting Information suggest that the PEVCD treatment incorporates a signiﬁcant amount of ﬂuorine onto the surface of the paint panel. The presence of ﬂuorine most likely contributes to the diminished surface energy and promotes sessile drop formation. As seen in Table 1, the relative amount of carbon near the surface of the ﬁlm dramatically decreased after the plasma treatment, while the concentration of oxygen and nitrogen in the polyurethane increases slightly. These results suggest that
hemical warfare agents (CWAs) are among the more lethal substances known to mankind.1 Not only do they pose an immediate threat to both civilian and military populations upon release2,3 but they also pose a threat via sorption on and into porous surfaces, creating equally lethal oﬀgassing and contact hazards over extended periods of time. Painted surfaces in particular, such as those found on vehicles and on buildings, provide a suﬃcient sink for agent uptake.4,5 Perﬂuoralkalation via plasma chemical vapor deposition (PECVD) is a well-known method for creating hydrophobic coatings.6 Furthermore, plasma based surface treatments have been used to alter surface and bulk properties of other materials.7−11 Herein we present a method for treating urethane-painted surfaces with a perﬂuoroalkane plasma, and the resulting impact on the agent resistant properties of the material. PECVD with perﬂuoroalkanes has been shown to modify many substrates, altering their surface, as generally shown in Figure 1. Scanning electron microscopy (SEM) images shown in Figure 2 illustrate the diﬀerence between treated and untreated panels. In both cases, materials are comprised of metal oxide and other particles dispersed throughout the urethane coating. The untreated coating exhibits large pores in the 1−30 μm range that could provide sites for CWA sorption, as determined by mercury porosimetry (Figure S1 in the Supporting Information). The plasma-treated sample, however, shows the eﬀects of two mechanisms. First, prior to plasma treatment the SEM image shows metal oxide pigments and ﬁllers were mostly © XXXX American Chemical Society
Received: January 26, 2015 Accepted: March 16, 2015
DOI: 10.1021/acsami.5b00790 ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
ACS Applied Materials & Interfaces
Figure 3. Two microliter VX drops on urethane painted surface for (a) plasma-treated surface after 12 s, (b) plasma-treated surface after 60 min, and (c) untreated surface after 12 s.
time point, but was estimated to be below 6° at 6 s and below 5° at 12 s (Figure 3c). Remaining agent studies were conducted to quantify resistance to agent sorption into the substrate due to the plasma treatment (detailed in the Supporting Information). Brieﬂy, as-obtained and PECVD-treated panels were equilibrated at 50% RH and 25 °C for 24 h, challenged with 2 μL of VX, and aged for 1 h in a covered in a Petri dish. Top-down images were collected at the end of the age period; typical examples of which are shown in Figure 4. Following the age
Figure 1. Schematic showing potential mechanisms of surface modiﬁcation using PECVD.
Figure 2. SEM images of untreated (left) and plasma-treated (right) urethane surfaces. The bar in the lower right corner shows a 5 μm scale.
Table 1. Near Surface Atomic % Values as Calculated via XPS Analysis; Trace Species from Paint Additives Were Excluded peak
C 1s O 1s N 1s F 1s
77.4 21.4 1.2 0.0
48.5 37.9 3.7 9.9
Figure 4. Two microliter VX drops on 2 in. diameter polyurethane painted panels 58 min after contamination: (a) untreated surface, (b) plasma-treated surface. The extent of liquid spreading is indicated by the red outline.
period, the panels were rinsed with 3 aliquots of 20 mL 18 MΩ deionized water, and then placed in a jar with 20 mL of isopropyl alcohol to extract remaining VX for 1 h. Both the rinsate and the extraction solvent were analyzed via an Agilent triple quadrupole LC/MS to determine the amount of VX that was rinsed oﬀ and the amount remaining in the panel after rinsing with low detection limits (